Influence of Deformation on the Kinetics of Phase ... The applied deformation enhances intragranular
Embed Size (px)
Transcript of Influence of Deformation on the Kinetics of Phase ... The applied deformation enhances intragranular
Vol. 7, No. 2, 2004 Influence of Deformation on the Kinetics of Phase Transformation in a Forging Steel During Warm Working 247Materials Research, Vol. 7, No. 2, 247-253, 2004. © 2004
Influence of Deformation on the Kinetics of
Phase Transformation in a Forging Steel During Warm Working
Mauro Aparecido Ferreira de Oliveiraa, Alberto Moreira Jorge Jrb, Oscar Balancinb*
aSIFCO S.A., Jundiaí - SP, Brazil bDepartment of Materials Engineering, Federal University of São Carlos, UFSCar
Rod. Washington Luiz, Km 235, 13565-905 São Carlos - SP, Brazil
Received: July 24, 2003; Revised: January 18, 2004
Dilatometric techniques were used to determine the start and finish transformation heating temperatures for a carbon steel (0.30% C - 1.5% Mn). The mechanical behavior of the steel was measured by torsion testing in the temperature range of 700 to 820 °C with holding times ranging from 1 to 30 min. The flow stress curves presented different shapes and stress levels. These differ- ences were attributed to the ferrite and pearlite, ferrite and austenite, and austenite strained struc- tures. When ferrite and pearlite were deformed together, the flow stress presented a hump with little straining; when the austenitic structure was deformed the shape of the flow stress curve was typical of materials having low stacking fault energy. The microstructural evolution observed by optical and scanning electron microscopy revealed that the evolution of the phase transformation was dependent on the testing temperatures, holding times and amount of straining. Comparisons were made on the kinetics of phase transformation with and without the application of plastic deformation, and evidence of strain-induced dynamic transformation was investigated.
Keywords: warm working, pearlite austenite transformation, flow stress curves
In recent years, increasing attention has been focused on steel working to improve the metallurgical features of formed parts and to produce forms as similar as possible to the net shape forms. One possible route to achieve these goals is deformation under warm working conditions, a tech- nique that provides greater dimensional precision than hot working, moderate surface oxidation, and improved me- chanical characteristics, obviating further machining and sometimes thermal treatments. However, warm working requires a more in-depth understanding of both the defor- mation process and the plastic behavior of materials, since this type of operation induces stronger mechanical efforts, often causing deformation in the intercritical region.
Manganese steels with a ferrite-pearlite starting micro- structure are usually applied in the production of forged components. Upon heating, pearlite becomes unstable above the eutectoid temperature (AC
1 ), whereas primary ferrite
does not revert completely to austenite except above AC 3
temperature. The formation of austenite from the ferrite- pearlite microstructure can be described as a sequence of three stages1. First, the pearlite regions are converted to car- bon supersaturated austenite. In this step, austenite nucle- ates heterogeneously at the boundary of pearlite colonies and/or ferrite-pearlite interfaces1,2,3. Austenite nuclei in pearlite grow when carbon atoms are transported by diffu- sion to the ferrite/austenite boundary from the austenite/cementite boundary through austenite and from the ferrite/cementite boundary through ferrite, transform- ing the ferritic lattice to austenitic lattice4. In the second stage, the austenite/ferrite boundaries move to decrease the amount of ferrite, until the equilibrium volume fraction of austenite is reached. At high temperatures within the intercritical domain, the growth of austenite into ferrite is controlled by carbon diffusion in the austenitic phase and, at lower temperatures, by manganese diffusion in ferrite3. At the final step, the equilibrium of the manganese content
248 Oliveira et al. Materials Research
in austenitic and ferritic phases is controlled by manganese diffusion in the austenite, which is a much slower process than in ferrite3.
It is well known that dislocation substructures formed during deformation increase the free energy and the number of potential nucleation sites accelerating diffusional-phase transformations5,6. One expects that dynamic phenomena should be enhanced by deformation assisted transforma- tions bringing about continual straining during transforma- tion7. The applied deformation enhances intragranular nu- cleation of the new phase within the untransformed grains promoting strain-induced transformation8,9. This is analo- gous to dynamic recrystallization. In the present work the transformation of a pearlite + ferrite microstructure into austenite during warm deformation of a medium carbon steel was studied. Attention was focused on the second stage of this transformation. The microstructural evolution of the ferrite into austenite transformation was quantified, seek- ing for evidences of strain-induced dynamic transformation.
2. Material and Experimental Procedures
The investigated material was a commercial medium carbon vanadium microalloyed forging steel whose chemi- cal composition is given in Table 1. To determine the con- tinuous-heating-transformation diagram, dilatometry tests were carried out using 2 mm diameter, 12 mm long sam- ples. These samples were heated at a rate of 1 to 10 °C/s.
Mechanical tests were carried out on a computerized hot torsion machine. The samples, having a 20 mm length and 6 mm diameter in the reduced central gage section, were heated in an infrared furnace coupled on the testing ma- chine. Chromel-alumel thermocouples were used for meas- uring the temperature. Throughout the tests, argon balanced with 2% hydrogen was continuously flushed through a quartz tube surrounding the sample. This tube was also used to inject water immediately, once the required strain had been attained, in order to freeze the high-temperature micro- structures for further observations. Data were collected by means of a software program that imposes parametric tests such as temperature, holding time and amount of straining.
Warm torsion tests were carried out after heating up the samples at a rate of 1.7 °C/s from room to testing tempera- tures (700, 720, 750, 780 and 820 °C). The specimens were held at these temperatures from 1 to 30 min and deformed at an equivalent strain rate of 1 s-1. In order to correlate the amount of deformation with the microstructural evolution, two different tests were performed in this investigation. In
one test, the samples were isothermally strained to fracture to determine the flow stress behavior. In the other, the tests were interrupted at selected strains and the samples were quenched by injecting water through the quartz tube imme- diately after deformation. After standard metallographic procedures, the microstructural evolution was observed by scanning electron and optical microscopy and the phases were quantified.
Start and finish transformation temperatures, under con- tinuous heating conditions determined by dilatometry tests, are illustrated in the continuous-heating-transformation dia- gram plotted in Fig. 1. These data indicate that the heating rate exerts a stronger influence on the finish temperature, when all the ferritic phase is exhausted, than on the start temperature at the beginning of pearlite dissolution.
To create a reference to analyze the role of the deforma- tion in the transformation kinetics, the evolution of the vol- ume fraction of ferrite as a function of the temperature with holding times of 0, 1, 3 and 30 min was measured in experi- ments conducted isothermally at 720, 750, 780 and 810 °C without any straining, as illustrated in Fig. 2. The results indicated that, regardless the holding time, no transforma- tion of ferrite into austenite was observed to occur at 720 °C. This transformation began at 750 °C, and the tendency for the ferritic phase to be consumed increased as the tempera-
Table 1. Chemical composition of the tested steel (wt.%).
C Mn Si P S Al V Ti N
0.30 1.52 0.64 0.016 0.033 0.024 0.1 0.024 0.017
Figure 1. Continuous-heating-transformation diagram determined by dilatometry.
Vol. 7, No. 2, 2004 Influence of Deformation on the Kinetics of Phase Transformation in a Forging Steel During Warm Working 249
ture rose. The entire volume fraction of ferrite was exhausted after long holding times at 810 °C.
Figure 3 illustrates some flow stress curves determined by isothermal continuous torsion tests. These curves repre- sent the different shapes and flow-stress levels presented by all the experiments carried out in this study. After a 1 min holding time at 700 °C, the flow curve shows a rapid work hardening to a hump, followed by an extensive flow-sof- tening region. The peak stress (437 MPa) was reached after a slight straining (ε = 0,14). At 820 °C, the flow stress rose in the initial work-hardening regime and also reached a maximum (213 MPa) before dropping to the steady state, albeit after greater straining (ε ~ 0.5). As can be seen, all the remaining curves displayed shapes and flow-stress lev- els intermediate to the ones described above, and the differ-
ences were temperature and holding time-dependent. Although the flow stress curves changed considerably,
these differences were significantly higher at the beginning of the straining, in the work-hardening regime. In order to delineate this stage on the flow stress curves, the evolution of peak stress and peak strain as a function of holding times before strai